#------------------------------------------------------------------------------
#$Date: 2016-03-26 22:48:34 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180519 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/88/7218885.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7218885
loop_
_publ_author_name
'Wang, Xiuli'
'Chang, Zhihan'
'Lin, Hongyan'
'Tian, Aixiang'
'Liu, Guocheng'
'Zhang, Juwen'
'Liu, Danna'
_publ_section_title
;
 Effect of polyoxoanions and amide group coordination modes on the
 assembly of polyoxometalate-based metal--organic complexes constructed
 from a semi-rigid bis-pyridyl-bis-amide ligand
;
_journal_issue                   4
_journal_name_full               CrystEngComm
_journal_page_first              895
_journal_paper_doi               10.1039/C4CE01933D
_journal_volume                  17
_journal_year                    2015
_chemical_formula_sum            'C32 H46 Cu2 N8 O51 Si W12'
_chemical_formula_weight         3720.14
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                106.758(2)
_cell_angle_beta                 108.015(2)
_cell_angle_gamma                108.944(2)
_cell_formula_units_Z            1
_cell_length_a                   12.3100(18)
_cell_length_b                   12.6680(18)
_cell_length_c                   13.816(2)
_cell_measurement_reflns_used    3077
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.9459
_cell_measurement_theta_min      2.6765
_cell_volume                     1747.6(4)
_computing_cell_refinement       'SMART (Bruker, 2001)'
_computing_data_collection       'SMART (Bruker, 2001)'
_computing_data_reduction        'SAINT+ (Bruker, 1999)'
_computing_molecular_graphics    'PLATON (Spek, 2003)'
_computing_publication_material  'SHELXTL (1998)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0428
_diffrn_reflns_av_unetI/netI     0.0766
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            8851
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         27.9459
_diffrn_reflns_theta_min         2.6765
_exptl_absorpt_coefficient_mu    20.375
_exptl_absorpt_correction_T_max  0.087
_exptl_absorpt_correction_T_min  0.008
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            BLUE
_exptl_crystal_density_diffrn    3.521
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       BLOCK
_exptl_crystal_F_000             1648
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.21
_exptl_crystal_size_min          0.12
_platon_squeeze_details
;
;
_refine_diff_density_max         4.088
_refine_diff_density_min         -4.628
_refine_diff_density_rms         0.471
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.050
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     499
_refine_ls_number_reflns         6098
_refine_ls_number_restraints     150
_refine_ls_restrained_S_all      1.065
_refine_ls_R_factor_all          0.0810
_refine_ls_R_factor_gt           0.0648
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1001P)²+36.9050P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1688
_refine_ls_wR_factor_ref         0.1778
_reflns_number_gt                4882
_reflns_number_total             8387
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c4ce01933d2.cif
_cod_data_source_block           complex3
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2935 2014-11-11 08:27:57Z andrius 

 Adding full bibliography for 7218883--7218886.cif.
;
_cod_database_code               7218885
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
W1 W 0.23625(7) 0.23008(7) -0.06076(6) 0.0193(2) Uani 1 1 d .
Si1 Si 0.5000 0.5000 0.0000 0.0103(13) Uani 1 2 d SU
O1W O 0.3757(16) 0.9666(15) 0.0978(14) 0.047(4) Uani 1 1 d .
N1 N 0.1157(14) 0.8124(16) 0.0216(13) 0.022(3) Uani 1 1 d .
C1 C 0.5224(19) 1.0493(19) 0.3534(16) 0.028(4) Uani 1 1 d .
H1A H 0.5318 0.9929 0.3004 0.033 Uiso 1 1 calc R
O1 O 0.3115(13) 0.7639(13) 0.1825(11) 0.028(3) Uani 1 1 d .
Cu1 Cu 0.2596(2) 0.9394(2) 0.1730(2) 0.0266(5) Uani 1 1 d .
W2 W 0.68615(7) 0.73522(7) 0.27862(7) 0.0242(2) Uani 1 1 d .
O2 O 0.5821(19) 0.2413(18) -0.0383(15) 0.067(6) Uani 1 1 d U
O2W O 0.227(2) 1.1012(18) 0.1585(16) 0.062(6) Uani 1 1 d .
N2 N 0.4051(17) 1.0479(17) 0.3249(15) 0.033(4) Uani 1 1 d .
C2 C -0.0029(19) 0.759(2) -0.1733(18) 0.030(5) Uani 1 1 d U
W3 W 0.55065(9) 0.28139(8) 0.09135(7) 0.0281(2) Uani 1 1 d .
N3 N 0.8179(18) 1.141(2) 0.4267(18) 0.050(6) Uani 1 1 d .
C3 C 0.0478(18) 0.6988(19) 0.0052(17) 0.028(4) Uani 1 1 d U
H3A H 0.0651 0.6784 0.0658 0.033 Uiso 1 1 calc R
O3W O 0.1373(13) 0.8989(16) 0.2372(12) 0.039(4) Uani 1 1 d .
O3 O 0.794(2) 1.108(3) 0.5701(18) 0.087(8) Uani 1 1 d .
O4W O 0.5000 0.5000 0.5000 0.079(9) Uani 1 2 d SU
W4 W 0.18398(7) 0.44596(8) -0.15789(7) 0.0241(2) Uani 1 1 d .
C4 C -0.0477(19) 0.610(2) -0.099(2) 0.044(6) Uani 1 1 d .
H4A H -0.0949 0.5311 -0.1070 0.052 Uiso 1 1 calc R
N4 N 0.046(2) 0.833(3) -0.307(2) 0.067(7) Uani 1 1 d U
O4 O 0.442(2) 0.398(2) 0.039(2) 0.017(5) Uani 0.50 1 d PU
O5 O 0.5843(18) 0.6050(19) 0.308(2) 0.074(6) Uani 1 1 d U
W5 W 0.36904(8) 0.67438(8) 0.12490(9) 0.0377(3) Uani 1 1 d U
C5 C -0.075(2) 0.636(2) -0.192(2) 0.041(6) Uani 1 1 d .
H5A H -0.1377 0.5754 -0.2632 0.050 Uiso 1 1 calc R
W6 W 0.42480(8) 0.45975(9) 0.21731(8) 0.0341(3) Uani 1 1 d .
O6 O 0.155(2) 0.3204(19) -0.1070(14) 0.057(5) Uani 1 1 d .
C6 C -0.036(2) 0.794(3) -0.269(2) 0.045(6) Uani 1 1 d .
O7 O 0.223(2) 0.5549(19) -0.0105(17) 0.070(6) Uani 1 1 d U
C7 C 0.395(2) 1.129(3) 0.402(2) 0.057(8) Uani 1 1 d .
H7A H 0.3149 1.1278 0.3855 0.069 Uiso 1 1 calc R
O8 O 0.3457(18) 0.5647(19) 0.190(2) 0.076(6) Uani 1 1 d U
C8 C 0.629(2) 1.130(2) 0.457(2) 0.043(6) Uani 1 1 d .
O9 O 0.5136(16) 0.3644(18) 0.2030(15) 0.057(5) Uani 1 1 d U
C9 C 0.754(2) 1.126(2) 0.4895(19) 0.043(6) Uani 1 1 d .
O10 O 0.2534(15) 0.1888(16) -0.1968(12) 0.040(4) Uani 1 1 d U
C10 C 0.493(3) 1.215(3) 0.505(3) 0.066(8) Uani 1 1 d U
H10A H 0.4824 1.2742 0.5542 0.079 Uiso 1 1 calc R
O11 O 0.3757(17) 0.1931(18) -0.0038(15) 0.061(5) Uani 1 1 d U
C11 C 0.945(3) 1.149(3) 0.469(2) 0.059(8) Uani 1 1 d .
H11A H 1.0075 1.2342 0.5178 0.071 Uiso 1 1 calc R
H11B H 0.9492 1.1014 0.5126 0.071 Uiso 1 1 calc R
O12 O 0.4026(19) 0.5639(19) -0.0278(18) 0.009(4) Uani 0.50 1 d PU
C12 C 0.090(2) 0.840(2) -0.0678(18) 0.034(5) Uani 1 1 d .
H12A H 0.1401 0.9195 -0.0561 0.041 Uiso 1 1 calc R
O13 O 0.505(2) 0.576(2) 0.1232(18) 0.011(5) Uani 0.50 1 d PU
C13 C 0.788(3) 1.191(3) 0.347(3) 0.065(8) Uani 1 1 d U
H13A H 0.6980 1.1707 0.3169 0.097 Uiso 1 1 calc R
H13B H 0.8376 1.2804 0.3842 0.097 Uiso 1 1 calc R
C14 C 0.614(3) 1.211(3) 0.536(3) 0.082(11) Uani 1 1 d .
H14A H 0.6809 1.2619 0.6082 0.099 Uiso 1 1 calc R
O14 O 0.638(2) 0.601(2) 0.086(2) 0.013(5) Uani 0.50 1 d PU
C15 C 0.973(3) 1.102(3) 0.379(3) 0.076(9) Uani 1 1 d U
H15A H 0.9172 1.0142 0.3355 0.091 Uiso 1 1 calc R
H15B H 1.0610 1.1154 0.4090 0.091 Uiso 1 1 calc R
O15 O 0.2763(17) 0.322(2) 0.0876(13) 0.063(6) Uani 1 1 d .
O16 O 0.7924(18) 0.6537(17) 0.2701(15) 0.050(5) Uani 1 1 d .
C16 C 0.185(3) 0.855(4) -0.261(3) 0.077(9) Uani 1 1 d U
H16A H 0.2416 0.9431 -0.2173 0.092 Uiso 1 1 calc R
H16B H 0.1987 0.8151 -0.2111 0.092 Uiso 1 1 calc R
O17 O 0.5424(18) 0.7652(19) 0.2287(19) 0.069(5) Uani 1 1 d U
O18 O 0.5737(15) 0.1758(14) 0.1327(15) 0.048(5) Uani 1 1 d .
O19 O 0.1123(17) 0.0983(15) -0.0908(19) 0.061(6) Uani 1 1 d .
O20 O 0.720(2) 0.413(2) 0.1714(19) 0.085(7) Uani 1 1 d U
O21 O 0.3878(17) 0.441(2) 0.3214(17) 0.064(5) Uani 1 1 d .
O22 O 0.0336(14) 0.4182(18) -0.2318(15) 0.048(5) Uani 1 1 d .
O23 O 0.7753(18) 0.8460(14) 0.4096(12) 0.046(4) Uani 1 1 d .
O24 O -0.1393(15) 0.801(2) -0.3010(14) 0.053(5) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O19 W1 O15 100.0(10) . .
O19 W1 O6 102.8(9) . .
O15 W1 O6 90.2(8) . .
O19 W1 O10 101.5(9) . .
O15 W1 O10 158.2(9) . .
O6 W1 O10 87.9(6) . .
O19 W1 O11 99.8(9) . .
O15 W1 O11 87.6(7) . .
O6 W1 O11 157.4(9) . .
O10 W1 O11 85.8(7) . .
O19 W1 O4 158.2(10) . .
O15 W1 O4 66.8(9) . .
O6 W1 O4 94.7(9) . .
O10 W1 O4 91.8(8) . .
O11 W1 O4 63.8(8) . .
O19 W1 O14 159.4(9) . 2_665
O15 W1 O14 96.0(9) . 2_665
O6 W1 O14 64.1(8) . 2_665
O10 W1 O14 63.8(8) . 2_665
O11 W1 O14 93.7(8) . 2_665
O4 W1 O14 42.2(8) . 2_665
O14 Si1 O14 179.999(3) . 2_665
O14 Si1 O4 65.8(11) . 2_665
O14 Si1 O4 114.2(11) 2_665 2_665
O14 Si1 O4 114.2(11) . .
O14 Si1 O4 65.8(11) 2_665 .
O4 Si1 O4 180.0(18) 2_665 .
O14 Si1 O12 69.6(11) . 2_665
O14 Si1 O12 110.4(11) 2_665 2_665
O4 Si1 O12 109.2(11) 2_665 2_665
O4 Si1 O12 70.8(11) . 2_665
O14 Si1 O12 110.4(11) . .
O14 Si1 O12 69.6(11) 2_665 .
O4 Si1 O12 70.8(11) 2_665 .
O4 Si1 O12 109.2(11) . .
O12 Si1 O12 179.999(3) 2_665 .
O14 Si1 O13 69.1(11) . .
O14 Si1 O13 110.9(11) 2_665 .
O4 Si1 O13 106.1(11) 2_665 .
O4 Si1 O13 73.9(11) . .
O12 Si1 O13 105.7(10) 2_665 .
O12 Si1 O13 74.3(10) . .
O14 Si1 O13 110.9(11) . 2_665
O14 Si1 O13 69.1(11) 2_665 2_665
O4 Si1 O13 73.9(11) 2_665 2_665
O4 Si1 O13 106.1(11) . 2_665
O12 Si1 O13 74.3(10) 2_665 2_665
O12 Si1 O13 105.7(10) . 2_665
O13 Si1 O13 179.999(2) . 2_665
C3 N1 C12 118.2(19) . .
C3 N1 Cu1 121.2(13) . .
C12 N1 Cu1 120.5(15) . .
N2 C1 C8 124(2) . .
N2 C1 H1A 118.1 . .
C8 C1 H1A 118.1 . .
O3W Cu1 N2 91.8(7) . .
O3W Cu1 N1 87.5(6) . .
N2 Cu1 N1 173.1(7) . .
O3W Cu1 O1W 175.4(7) . .
N2 Cu1 O1W 91.9(7) . .
N1 Cu1 O1W 88.4(7) . .
O3W Cu1 O2W 92.9(7) . .
N2 Cu1 O2W 91.6(8) . .
N1 Cu1 O2W 95.3(7) . .
O1W Cu1 O2W 89.6(7) . .
O23 W2 O10 101.9(8) . 2_665
O23 W2 O17 102.5(9) . .
O10 W2 O17 87.6(8) 2_665 .
O23 W2 O16 100.1(8) . .
O10 W2 O16 87.9(6) 2_665 .
O17 W2 O16 157.4(9) . .
O23 W2 O5 99.6(9) . .
O10 W2 O5 158.5(9) 2_665 .
O17 W2 O5 88.4(8) . .
O16 W2 O5 87.7(7) . .
O23 W2 O13 157.9(9) . .
O10 W2 O13 94.6(8) 2_665 .
O17 W2 O13 63.3(8) . .
O16 W2 O13 95.0(8) . .
O5 W2 O13 64.9(9) . .
O23 W2 O14 157.2(8) . .
O10 W2 O14 62.3(7) 2_665 .
O17 W2 O14 93.6(9) . .
O16 W2 O14 64.8(7) . .
O5 W2 O14 96.8(9) . .
O13 W2 O14 44.8(7) . .
W3 O2 W5 136.2(12) . 2_665
C7 N2 C1 117(2) . .
C7 N2 Cu1 120.7(17) . .
C1 N2 Cu1 122.6(14) . .
C12 C2 C5 118(2) . .
C12 C2 C6 124(2) . .
C5 C2 C6 119(2) . .
O18 W3 O11 99.7(8) . .
O18 W3 O9 100.7(9) . .
O11 W3 O9 88.6(8) . .
O18 W3 O20 100.4(10) . .
O11 W3 O20 159.9(10) . .
O9 W3 O20 87.9(9) . .
O18 W3 O2 99.7(10) . .
O11 W3 O2 88.9(8) . .
O9 W3 O2 159.5(9) . .
O20 W3 O2 87.5(8) . .
O18 W3 O12 155.9(8) . 2_665
O11 W3 O12 97.8(8) . 2_665
O9 W3 O12 96.1(8) . 2_665
O20 W3 O12 63.0(9) . 2_665
O2 W3 O12 64.1(8) . 2_665
O18 W3 O4 157.5(8) . .
O11 W3 O4 63.1(8) . .
O9 W3 O4 66.2(8) . .
O20 W3 O4 97.5(10) . .
O2 W3 O4 94.6(9) . .
O12 W3 O4 46.5(8) 2_665 .
C9 N3 C13 123(2) . .
C9 N3 C11 117.0(18) . .
C13 N3 C11 117(2) . .
N1 C3 C4 122(2) . .
N1 C3 H3A 119.1 . .
C4 C3 H3A 119.1 . .
O22 W4 O16 100.4(8) . 2_665
O22 W4 O6 101.0(8) . .
O16 W4 O6 87.9(7) 2_665 .
O22 W4 O20 101.8(10) . 2_665
O16 W4 O20 89.8(8) 2_665 2_665
O6 W4 O20 157.1(10) . 2_665
O22 W4 O7 101.6(9) . .
O16 W4 O7 157.9(9) 2_665 .
O6 W4 O7 86.1(8) . .
O20 W4 O7 87.6(9) 2_665 .
O22 W4 O12 157.4(8) . .
O16 W4 O12 96.2(8) 2_665 .
O6 W4 O12 94.8(8) . .
O20 W4 O12 62.8(9) 2_665 .
O7 W4 O12 63.2(8) . .
O22 W4 O14 157.7(8) . 2_665
O16 W4 O14 66.0(8) 2_665 2_665
O6 W4 O14 62.4(8) . 2_665
O20 W4 O14 96.0(10) 2_665 2_665
O7 W4 O14 92.4(9) . 2_665
O12 W4 O14 44.9(7) . 2_665
C3 C4 C5 121(2) . .
C3 C4 H4A 119.6 . .
C5 C4 H4A 119.6 . .
C6 N4 C15 122(3) . 2_675
C6 N4 C16 127(2) . .
C15 N4 C16 109(2) 2_675 .
Si1 O4 O14 56.1(11) . 2_665
Si1 O4 W1 126.3(13) . .
O14 O4 W1 70.2(10) 2_665 .
Si1 O4 W3 121.7(12) . .
O14 O4 W3 134.3(15) 2_665 .
W1 O4 W3 95.5(8) . .
Si1 O4 W6 119.8(12) . .
O14 O4 W6 131.1(14) 2_665 .
W1 O4 W6 93.5(8) . .
W3 O4 W6 91.7(8) . .
W6 O5 W2 133.8(13) . .
O1 W5 O8 100.9(9) . .
O1 W5 O17 99.8(8) . .
O8 W5 O17 90.7(8) . .
O1 W5 O7 101.5(8) . .
O8 W5 O7 90.5(9) . .
O17 W5 O7 157.9(10) . .
O1 W5 O2 97.3(8) . 2_665
O8 W5 O2 161.8(10) . 2_665
O17 W5 O2 85.0(9) . 2_665
O7 W5 O2 86.9(8) . 2_665
O1 W5 O13 156.3(7) . .
O8 W5 O13 67.1(9) . .
O17 W5 O13 61.5(8) . .
O7 W5 O13 99.0(9) . .
O2 W5 O13 95.4(9) 2_665 .
O1 W5 O12 153.5(7) . .
O8 W5 O12 100.2(9) . .
O17 W5 O12 95.7(9) . .
O7 W5 O12 62.4(8) . .
O2 W5 O12 62.7(8) 2_665 .
O13 W5 O12 49.5(7) . .
C4 C5 C2 117(2) . .
C4 C5 H5A 121.5 . .
C2 C5 H5A 121.5 . .
O21 W6 O9 101.3(10) . .
O21 W6 O5 98.5(10) . .
O9 W6 O5 89.5(8) . .
O21 W6 O15 100.1(9) . .
O9 W6 O15 87.8(7) . .
O5 W6 O15 161.4(10) . .
O21 W6 O8 98.7(10) . .
O9 W6 O8 160.1(10) . .
O5 W6 O8 88.1(8) . .
O15 W6 O8 88.2(8) . .
O21 W6 O13 155.2(9) . .
O9 W6 O13 95.5(8) . .
O5 W6 O13 63.3(9) . .
O15 W6 O13 98.6(8) . .
O8 W6 O13 65.8(9) . .
O21 W6 O4 157.4(9) . .
O9 W6 O4 64.9(8) . .
O5 W6 O4 99.0(9) . .
O15 W6 O4 63.3(8) . .
O8 W6 O4 96.0(9) . .
O13 W6 O4 47.3(8) . .
W1 O6 W4 139.2(11) . .
O24 C6 N4 120(2) . .
O24 C6 C2 117.1(19) . .
N4 C6 C2 122(2) . .
W5 O7 W4 138.4(11) . .
N2 C7 C10 125(2) . .
N2 C7 H7A 117.7 . .
C10 C7 H7A 117.7 . .
W5 O8 W6 133.8(13) . .
C14 C8 C1 118(2) . .
C14 C8 C9 119(2) . .
C1 C8 C9 123(2) . .
W3 O9 W6 137.0(10) . .
O3 C9 N3 122(2) . .
O3 C9 C8 118(2) . .
N3 C9 C8 120(2) . .
W2 O10 W1 140.0(9) 2_665 .
C7 C10 C14 118(3) . .
C7 C10 H10A 121.0 . .
C14 C10 H10A 121.0 . .
W3 O11 W1 137.1(11) . .
C15 C11 N3 111(2) . .
C15 C11 H11A 109.4 . .
N3 C11 H11A 109.4 . .
C15 C11 H11B 109.4 . .
N3 C11 H11B 109.4 . .
H11A C11 H11B 108.0 . .
Si1 O12 W3 121.0(11) . 2_665
Si1 O12 W4 122.4(11) . .
W3 O12 W4 97.1(7) 2_665 .
Si1 O12 W5 117.8(10) . .
W3 O12 W5 96.8(8) 2_665 .
W4 O12 W5 95.9(8) . .
N1 C12 C2 124(2) . .
N1 C12 H12A 117.8 . .
C2 C12 H12A 117.8 . .
Si1 O13 W2 125.1(11) . .
Si1 O13 W5 118.3(11) . .
W2 O13 W5 96.8(8) . .
Si1 O13 W6 119.0(11) . .
W2 O13 W6 97.9(8) . .
W5 O13 W6 93.2(8) . .
C16 C13 N3 111(3) 2_675 .
C16 C13 H13A 109.4 2_675 .
N3 C13 H13A 109.4 . .
C16 C13 H13B 109.4 2_675 .
N3 C13 H13B 109.4 . .
H13A C13 H13B 108.0 . .
C8 C14 C10 119(3) . .
C8 C14 H14A 120.7 . .
C10 C14 H14A 120.7 . .
Si1 O14 O4 58.0(11) . 2_665
Si1 O14 W1 125.7(12) . 2_665
O4 O14 W1 67.6(10) 2_665 2_665
Si1 O14 W4 123.0(12) . 2_665
O4 O14 W4 134.3(15) 2_665 2_665
W1 O14 W4 93.6(7) 2_665 2_665
Si1 O14 W2 121.0(12) . .
O4 O14 W2 129.0(14) 2_665 .
W1 O14 W2 93.1(8) 2_665 .
W4 O14 W2 91.6(7) 2_665 .
C11 C15 N4 109(3) . 2_675
C11 C15 H15A 109.8 . .
N4 C15 H15A 109.8 2_675 .
C11 C15 H15B 109.8 . .
N4 C15 H15B 109.8 2_675 .
H15A C15 H15B 108.3 . .
W1 O15 W6 136.2(12) . .
W4 O16 W2 137.3(10) 2_665 .
C13 C16 N4 110(3) 2_675 .
C13 C16 H16A 109.7 2_675 .
N4 C16 H16A 109.7 . .
C13 C16 H16B 109.7 2_675 .
N4 C16 H16B 109.7 . .
H16A C16 H16B 108.2 . .
W5 O17 W2 137.7(12) . .
W4 O20 W3 137.0(15) 2_665 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O19 1.686(15) .
W1 O15 1.851(15) .
W1 O6 1.867(14) .
W1 O10 1.897(14) .
W1 O11 1.920(15) .
W1 O4 2.34(2) .
W1 O14 2.39(2) 2_665
Si1 O14 1.55(2) .
Si1 O14 1.55(2) 2_665
Si1 O4 1.58(2) 2_665
Si1 O4 1.58(2) .
Si1 O12 1.66(2) 2_665
Si1 O12 1.66(2) .
Si1 O13 1.66(2) .
Si1 O13 1.66(2) 2_665
O1W Cu1 2.011(15) .
N1 C3 1.32(3) .
N1 C12 1.35(2) .
N1 Cu1 2.005(16) .
C1 N2 1.37(3) .
C1 C8 1.39(3) .
C1 H1A 0.9300 .
O1 W5 1.665(13) .
Cu1 O3W 1.976(14) .
Cu1 N2 1.978(19) .
Cu1 O2W 2.264(16) .
W2 O23 1.660(14) .
W2 O10 1.856(15) 2_665
W2 O17 1.893(18) .
W2 O16 1.922(15) .
W2 O5 1.95(2) .
W2 O13 2.30(2) .
W2 O14 2.47(2) .
O2 W3 1.909(16) .
O2 W5 1.924(17) 2_665
N2 C7 1.33(3) .
C2 C12 1.35(3) .
C2 C5 1.42(3) .
C2 C6 1.49(3) .
W3 O18 1.668(14) .
W3 O11 1.859(18) .
W3 O9 1.872(17) .
W3 O20 1.90(2) .
W3 O12 2.349(19) 2_665
W3 O4 2.41(2) .
N3 C9 1.35(3) .
N3 C13 1.43(3) .
N3 C11 1.45(3) .
C3 C4 1.37(3) .
C3 H3A 0.9300 .
O3 C9 1.19(3) .
W4 O22 1.671(14) .
W4 O16 1.863(17) 2_665
W4 O6 1.892(16) .
W4 O20 1.89(2) 2_665
W4 O7 1.90(2) .
W4 O12 2.36(2) .
W4 O14 2.45(2) 2_665
C4 C5 1.39(3) .
C4 H4A 0.9300 .
N4 C6 1.30(3) .
N4 C15 1.47(4) 2_675
N4 C16 1.53(4) .
O4 O14 1.70(3) 2_665
O4 W6 2.46(2) .
O5 W6 1.90(2) .
W5 O8 1.851(19) .
W5 O17 1.870(19) .
W5 O7 1.88(2) .
W5 O2 1.924(17) 2_665
W5 O13 2.40(2) .
W5 O12 2.41(2) .
C5 H5A 0.9300 .
W6 O21 1.691(19) .
W6 O9 1.883(15) .
W6 O15 1.923(18) .
W6 O8 1.941(17) .
W6 O13 2.40(2) .
C6 O24 1.25(3) .
C7 C10 1.36(4) .
C7 H7A 0.9300 .
C8 C14 1.36(4) .
C8 C9 1.49(3) .
O10 W2 1.856(15) 2_665
C10 C14 1.44(4) .
C10 H10A 0.9300 .
C11 C15 1.40(4) .
C11 H11A 0.9700 .
C11 H11B 0.9700 .
O12 W3 2.349(19) 2_665
C12 H12A 0.9300 .
C13 C16 1.35(4) 2_675
C13 H13A 0.9700 .
C13 H13B 0.9700 .
C14 H14A 0.9300 .
O14 O4 1.70(3) 2_665
O14 W1 2.39(2) 2_665
O14 W4 2.45(2) 2_665
C15 N4 1.47(4) 2_675
C15 H15A 0.9700 .
C15 H15B 0.9700 .
O16 W4 1.863(17) 2_665
C16 C13 1.35(4) 2_675
C16 H16A 0.9700 .
C16 H16B 0.9700 .
O20 W4 1.89(2) 2_665
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
C3 N1 Cu1 O3W -52.6(15) . .
C12 N1 Cu1 O3W 130.9(15) . .
C3 N1 Cu1 N2 32(6) . .
C12 N1 Cu1 N2 -144(5) . .
C3 N1 Cu1 O1W 125.3(15) . .
C12 N1 Cu1 O1W -51.2(15) . .
C3 N1 Cu1 O2W -145.2(14) . .
C12 N1 Cu1 O2W 38.3(15) . .
C8 C1 N2 C7 0(3) . .
C8 C1 N2 Cu1 175.8(16) . .
O3W Cu1 N2 C7 -45.9(19) . .
N1 Cu1 N2 C7 -131(5) . .
O1W Cu1 N2 C7 136.7(19) . .
O2W Cu1 N2 C7 47.0(19) . .
O3W Cu1 N2 C1 138.3(16) . .
N1 Cu1 N2 C1 54(6) . .
O1W Cu1 N2 C1 -39.1(16) . .
O2W Cu1 N2 C1 -128.8(16) . .
W5 O2 W3 O18 -157.8(16) 2_665 .
W5 O2 W3 O11 102.5(17) 2_665 .
W5 O2 W3 O9 20(3) 2_665 .
W5 O2 W3 O20 -57.7(18) 2_665 .
W5 O2 W3 O12 3.4(14) 2_665 2_665
W5 O2 W3 O4 39.7(17) 2_665 .
C12 N1 C3 C4 -1(3) . .
Cu1 N1 C3 C4 -177.6(16) . .
N1 C3 C4 C5 1(3) . .
O14 Si1 O4 O14 179.999(4) . 2_665
O4 Si1 O4 O14 122(35) 2_665 2_665
O12 Si1 O4 O14 -124.1(14) 2_665 2_665
O12 Si1 O4 O14 55.9(14) . 2_665
O13 Si1 O4 O14 122.4(13) . 2_665
O13 Si1 O4 O14 -57.6(13) 2_665 2_665
O14 Si1 O4 W1 178.7(13) . .
O14 Si1 O4 W1 -1.3(13) 2_665 .
O4 Si1 O4 W1 120(34) 2_665 .
O12 Si1 O4 W1 -125.3(17) 2_665 .
O12 Si1 O4 W1 54.7(17) . .
O13 Si1 O4 W1 121.1(17) . .
O13 Si1 O4 W1 -58.9(17) 2_665 .
O14 Si1 O4 W3 -55.0(17) . .
O14 Si1 O4 W3 125.0(17) 2_665 .
O4 Si1 O4 W3 -113(34) 2_665 .
O12 Si1 O4 W3 1.0(12) 2_665 .
O12 Si1 O4 W3 -179.0(12) . .
O13 Si1 O4 W3 -112.5(15) . .
O13 Si1 O4 W3 67.5(15) 2_665 .
O14 Si1 O4 W6 58.1(16) . .
O14 Si1 O4 W6 -121.9(16) 2_665 .
O4 Si1 O4 W6 0(34) 2_665 .
O12 Si1 O4 W6 114.1(15) 2_665 .
O12 Si1 O4 W6 -65.9(15) . .
O13 Si1 O4 W6 0.6(11) . .
O13 Si1 O4 W6 -179.4(11) 2_665 .
O19 W1 O4 Si1 175.4(15) . .
O15 W1 O4 Si1 -128.9(18) . .
O6 W1 O4 Si1 -40.7(16) . .
O10 W1 O4 Si1 47.3(16) . .
O11 W1 O4 Si1 131.8(18) . .
O14 W1 O4 Si1 1.1(12) 2_665 .
O19 W1 O4 O14 174.3(19) . 2_665
O15 W1 O4 O14 -130.0(13) . 2_665
O6 W1 O4 O14 -41.8(12) . 2_665
O10 W1 O4 O14 46.2(11) . 2_665
O11 W1 O4 O14 130.7(14) . 2_665
O19 W1 O4 W3 39(2) . .
O15 W1 O4 W3 94.7(9) . .
O6 W1 O4 W3 -177.2(7) . .
O10 W1 O4 W3 -89.1(8) . .
O11 W1 O4 W3 -4.6(7) . .
O14 W1 O4 W3 -135.3(14) 2_665 .
O19 W1 O4 W6 -53(2) . .
O15 W1 O4 W6 2.6(7) . .
O6 W1 O4 W6 90.8(8) . .
O10 W1 O4 W6 178.9(7) . .
O11 W1 O4 W6 -96.6(9) . .
O14 W1 O4 W6 132.6(14) 2_665 .
O18 W3 O4 Si1 -177.7(16) . .
O11 W3 O4 Si1 -134.5(17) . .
O9 W3 O4 Si1 124.3(16) . .
O20 W3 O4 Si1 40.0(15) . .
O2 W3 O4 Si1 -48.1(15) . .
O12 W3 O4 Si1 -0.9(11) 2_665 .
O18 W3 O4 O14 -106(3) . 2_665
O11 W3 O4 O14 -62.8(19) . 2_665
O9 W3 O4 O14 -164(2) . 2_665
O20 W3 O4 O14 111.7(19) . 2_665
O2 W3 O4 O14 24(2) . 2_665
O12 W3 O4 O14 70.8(19) 2_665 2_665
O18 W3 O4 W1 -38(2) . .
O11 W3 O4 W1 4.8(8) . .
O9 W3 O4 W1 -96.4(9) . .
O20 W3 O4 W1 179.3(8) . .
O2 W3 O4 W1 91.2(8) . .
O12 W3 O4 W1 138.4(13) 2_665 .
O18 W3 O4 W6 55(2) . .
O11 W3 O4 W6 98.5(9) . .
O9 W3 O4 W6 -2.7(7) . .
O20 W3 O4 W6 -87.0(8) . .
O2 W3 O4 W6 -175.1(7) . .
O12 W3 O4 W6 -127.9(12) 2_665 .
O23 W2 O5 W6 159.2(15) . .
O10 W2 O5 W6 -23(3) 2_665 .
O17 W2 O5 W6 56.8(16) . .
O16 W2 O5 W6 -100.9(15) . .
O13 W2 O5 W6 -4.3(13) . .
O14 W2 O5 W6 -36.7(16) . .
C3 C4 C5 C2 -2(3) . .
C12 C2 C5 C4 3(3) . .
C6 C2 C5 C4 -175(2) . .
W2 O5 W6 O21 -158.0(15) . .
W2 O5 W6 O9 100.7(15) . .
W2 O5 W6 O15 19(3) . .
W2 O5 W6 O8 -59.5(16) . .
W2 O5 W6 O13 4.2(13) . .
W2 O5 W6 O4 36.2(16) . .
Si1 O4 W6 O21 178.7(17) . .
O14 O4 W6 O21 109(3) 2_665 .
W1 O4 W6 O21 43(2) . .
W3 O4 W6 O21 -53(2) . .
Si1 O4 W6 O9 -125.8(15) . .
O14 O4 W6 O9 165(2) 2_665 .
W1 O4 W6 O9 98.2(10) . .
W3 O4 W6 O9 2.7(7) . .
Si1 O4 W6 O5 -40.6(14) . .
O14 O4 W6 O5 -109.9(18) 2_665 .
W1 O4 W6 O5 -176.6(8) . .
W3 O4 W6 O5 87.8(8) . .
Si1 O4 W6 O15 133.4(16) . .
O14 O4 W6 O15 64.1(18) 2_665 .
W1 O4 W6 O15 -2.6(7) . .
W3 O4 W6 O15 -98.2(9) . .
Si1 O4 W6 O8 48.4(14) . .
O14 O4 W6 O8 -20.9(19) 2_665 .
W1 O4 W6 O8 -87.6(9) . .
W3 O4 W6 O8 176.9(8) . .
Si1 O4 W6 O13 -0.5(10) . .
O14 O4 W6 O13 -69.8(18) 2_665 .
W1 O4 W6 O13 -136.5(12) . .
W3 O4 W6 O13 127.9(12) . .
O19 W1 O6 W4 -153.9(16) . .
O15 W1 O6 W4 105.7(17) . .
O10 W1 O6 W4 -52.5(16) . .
O11 W1 O6 W4 22(3) . .
O4 W1 O6 W4 39.0(17) . .
O14 W1 O6 W4 9.2(14) 2_665 .
O22 W4 O6 W1 155.0(16) . .
O16 W4 O6 W1 54.8(16) 2_665 .
O20 W4 O6 W1 -30(3) 2_665 .
O7 W4 O6 W1 -103.9(17) . .
O12 W4 O6 W1 -41.3(17) . .
O14 W4 O6 W1 -9.1(14) 2_665 .
C15 N4 C6 O24 6(5) 2_675 .
C16 N4 C6 O24 167(3) . .
C15 N4 C6 C2 -164(3) 2_675 .
C16 N4 C6 C2 -3(5) . .
C12 C2 C6 O24 -107(3) . .
C5 C2 C6 O24 71(3) . .
C12 C2 C6 N4 63(4) . .
C5 C2 C6 N4 -120(3) . .
O1 W5 O7 W4 154.1(16) . .
O8 W5 O7 W4 -104.7(18) . .
O17 W5 O7 W4 -11(4) . .
O2 W5 O7 W4 57.3(18) 2_665 .
O13 W5 O7 W4 -37.7(18) . .
O12 W5 O7 W4 -3.4(15) . .
O22 W4 O7 W5 -158.7(17) . .
O16 W4 O7 W5 26(3) 2_665 .
O6 W4 O7 W5 100.9(18) . .
O20 W4 O7 W5 -57.2(18) 2_665 .
O12 W4 O7 W5 3.5(15) . .
O14 W4 O7 W5 38.7(18) 2_665 .
C1 N2 C7 C10 2(4) . .
Cu1 N2 C7 C10 -174(2) . .
O1 W5 O8 W6 -157.2(15) . .
O17 W5 O8 W6 -57.0(17) . .
O7 W5 O8 W6 101.0(17) . .
O2 W5 O8 W6 19(4) 2_665 .
O13 W5 O8 W6 1.4(14) . .
O12 W5 O8 W6 38.9(17) . .
O21 W6 O8 W5 158.4(16) . .
O9 W6 O8 W5 -23(4) . .
O5 W6 O8 W5 60.1(18) . .
O15 W6 O8 W5 -101.7(17) . .
O13 W6 O8 W5 -1.4(14) . .
O4 W6 O8 W5 -38.8(17) . .
N2 C1 C8 C14 2(4) . .
N2 C1 C8 C9 176(2) . .
O18 W3 O9 W6 -155.6(15) . .
O11 W3 O9 W6 -56.0(17) . .
O20 W3 O9 W6 104.2(18) . .
O2 W3 O9 W6 27(3) . .
O12 W3 O9 W6 41.7(17) 2_665 .
O4 W3 O9 W6 5.1(14) . .
O21 W6 O9 W3 156.2(16) . .
O5 W6 O9 W3 -105.2(17) . .
O15 W6 O9 W3 56.3(17) . .
O8 W6 O9 W3 -22(4) . .
O13 W6 O9 W3 -42.1(17) . .
O4 W6 O9 W3 -5.0(14) . .
C13 N3 C9 O3 -165(3) . .
C11 N3 C9 O3 -7(4) . .
C13 N3 C9 C8 15(4) . .
C11 N3 C9 C8 174(3) . .
C14 C8 C9 O3 55(4) . .
C1 C8 C9 O3 -120(3) . .
C14 C8 C9 N3 -126(3) . .
C1 C8 C9 N3 60(3) . .
O19 W1 O10 W2 154.7(14) . 2_665
O15 W1 O10 W2 -33(3) . 2_665
O6 W1 O10 W2 52.0(14) . 2_665
O11 W1 O10 W2 -106.2(14) . 2_665
O4 W1 O10 W2 -42.7(14) . 2_665
O14 W1 O10 W2 -10.0(12) 2_665 2_665
N2 C7 C10 C14 -5(5) . .
O18 W3 O11 W1 156.0(16) . .
O9 W3 O11 W1 55.4(17) . .
O20 W3 O11 W1 -25(3) . .
O2 W3 O11 W1 -104.3(17) . .
O12 W3 O11 W1 -40.6(17) 2_665 .
O4 W3 O11 W1 -8.5(14) . .
O19 W1 O11 W3 -156.2(16) . .
O15 W1 O11 W3 -56.5(17) . .
O6 W1 O11 W3 28(3) . .
O10 W1 O11 W3 102.7(17) . .
O4 W1 O11 W3 8.7(14) . .
O14 W1 O11 W3 39.4(17) 2_665 .
C9 N3 C11 C15 150(3) . .
C13 N3 C11 C15 -50(4) . .
O14 Si1 O12 W3 54.7(15) . 2_665
O14 Si1 O12 W3 -125.3(15) 2_665 2_665
O4 Si1 O12 W3 1.0(12) 2_665 2_665
O4 Si1 O12 W3 -179.0(12) . 2_665
O12 Si1 O12 W3 -29(10) 2_665 2_665
O13 Si1 O12 W3 114.7(14) . 2_665
O13 Si1 O12 W3 -65.3(14) 2_665 2_665
O14 Si1 O12 W4 178.2(12) . .
O14 Si1 O12 W4 -1.8(12) 2_665 .
O4 Si1 O12 W4 124.4(15) 2_665 .
O4 Si1 O12 W4 -55.6(15) . .
O12 Si1 O12 W4 94(10) 2_665 .
O13 Si1 O12 W4 -121.8(14) . .
O13 Si1 O12 W4 58.2(14) 2_665 .
O14 Si1 O12 W5 -63.5(14) . .
O14 Si1 O12 W5 116.5(14) 2_665 .
O4 Si1 O12 W5 -117.3(14) 2_665 .
O4 Si1 O12 W5 62.7(14) . .
O12 Si1 O12 W5 -148(10) 2_665 .
O13 Si1 O12 W5 -3.5(10) . .
O13 Si1 O12 W5 176.5(10) 2_665 .
O22 W4 O12 Si1 177.9(14) . .
O16 W4 O12 Si1 -44.9(13) 2_665 .
O6 W4 O12 Si1 43.5(13) . .
O20 W4 O12 Si1 -131.5(16) 2_665 .
O7 W4 O12 Si1 126.7(15) . .
O14 W4 O12 Si1 1.5(10) 2_665 .
O22 W4 O12 W3 -48(2) . 2_665
O16 W4 O12 W3 89.0(8) 2_665 2_665
O6 W4 O12 W3 177.4(7) . 2_665
O20 W4 O12 W3 2.4(8) 2_665 2_665
O7 W4 O12 W3 -99.5(10) . 2_665
O14 W4 O12 W3 135.4(13) 2_665 2_665
O22 W4 O12 W5 49(2) . .
O16 W4 O12 W5 -173.3(6) 2_665 .
O6 W4 O12 W5 -85.0(7) . .
O20 W4 O12 W5 100.1(10) 2_665 .
O7 W4 O12 W5 -1.8(8) . .
O14 W4 O12 W5 -126.9(12) 2_665 .
O1 W5 O12 Si1 173.1(11) . .
O8 W5 O12 Si1 -44.6(12) . .
O17 W5 O12 Si1 47.2(12) . .
O7 W5 O12 Si1 -129.8(14) . .
O2 W5 O12 Si1 128.6(14) 2_665 .
O13 W5 O12 Si1 3.1(9) . .
O1 W5 O12 W3 42.6(18) . 2_665
O8 W5 O12 W3 -175.1(7) . 2_665
O17 W5 O12 W3 -83.3(8) . 2_665
O7 W5 O12 W3 99.7(10) . 2_665
O2 W5 O12 W3 -1.9(8) 2_665 2_665
O13 W5 O12 W3 -127.4(11) . 2_665
O1 W5 O12 W4 -55.3(17) . .
O8 W5 O12 W4 87.1(8) . .
O17 W5 O12 W4 178.9(7) . .
O7 W5 O12 W4 1.8(8) . .
O2 W5 O12 W4 -99.7(9) 2_665 .
O13 W5 O12 W4 134.7(11) . .
C3 N1 C12 C2 2(3) . .
Cu1 N1 C12 C2 178.4(16) . .
C5 C2 C12 N1 -3(3) . .
C6 C2 C12 N1 175.1(19) . .
O14 Si1 O13 W2 0.4(12) . .
O14 Si1 O13 W2 -179.6(12) 2_665 .
O4 Si1 O13 W2 -55.1(16) 2_665 .
O4 Si1 O13 W2 124.9(16) . .
O12 Si1 O13 W2 60.8(15) 2_665 .
O12 Si1 O13 W2 -119.2(15) . .
O13 Si1 O13 W2 46(9) 2_665 .
O14 Si1 O13 W5 123.2(14) . .
O14 Si1 O13 W5 -56.8(14) 2_665 .
O4 Si1 O13 W5 67.7(14) 2_665 .
O4 Si1 O13 W5 -112.3(14) . .
O12 Si1 O13 W5 -176.4(10) 2_665 .
O12 Si1 O13 W5 3.6(10) . .
O13 Si1 O13 W5 169(9) 2_665 .
O14 Si1 O13 W6 -125.0(14) . .
O14 Si1 O13 W6 55.0(14) 2_665 .
O4 Si1 O13 W6 179.4(11) 2_665 .
O4 Si1 O13 W6 -0.6(11) . .
O12 Si1 O13 W6 -64.7(13) 2_665 .
O12 Si1 O13 W6 115.3(13) . .
O13 Si1 O13 W6 -79(9) 2_665 .
O23 W2 O13 Si1 -179.6(14) . .
O10 W2 O13 Si1 41.9(14) 2_665 .
O17 W2 O13 Si1 126.9(16) . .
O16 W2 O13 Si1 -46.4(14) . .
O5 W2 O13 Si1 -131.5(16) . .
O14 W2 O13 Si1 -0.3(10) . .
O23 W2 O13 W5 49(2) . .
O10 W2 O13 W5 -89.9(8) 2_665 .
O17 W2 O13 W5 -4.9(8) . .
O16 W2 O13 W5 -178.2(7) . .
O5 W2 O13 W5 96.7(9) . .
O14 W2 O13 W5 -132.1(13) . .
O23 W2 O13 W6 -46(2) . .
O10 W2 O13 W6 175.8(7) 2_665 .
O17 W2 O13 W6 -99.1(10) . .
O16 W2 O13 W6 87.6(7) . .
O5 W2 O13 W6 2.5(7) . .
O14 W2 O13 W6 133.6(12) . .
O1 W5 O13 Si1 -172.0(12) . .
O8 W5 O13 Si1 124.7(15) . .
O17 W5 O13 Si1 -131.1(15) . .
O7 W5 O13 Si1 38.0(13) . .
O2 W5 O13 Si1 -49.7(13) 2_665 .
O12 W5 O13 Si1 -3.1(9) . .
O1 W5 O13 W2 -36(2) . .
O8 W5 O13 W2 -99.1(10) . .
O17 W5 O13 W2 5.1(8) . .
O7 W5 O13 W2 174.1(7) . .
O2 W5 O13 W2 86.4(8) 2_665 .
O12 W5 O13 W2 133.0(12) . .
O1 W5 O13 W6 62.5(19) . .
O8 W5 O13 W6 -0.8(8) . .
O17 W5 O13 W6 103.4(10) . .
O7 W5 O13 W6 -87.6(8) . .
O2 W5 O13 W6 -175.3(7) 2_665 .
O12 W5 O13 W6 -128.7(11) . .
O21 W6 O13 Si1 -178.8(15) . .
O9 W6 O13 Si1 48.4(12) . .
O5 W6 O13 Si1 135.1(15) . .
O15 W6 O13 Si1 -40.1(13) . .
O8 W6 O13 Si1 -124.2(14) . .
O4 W6 O13 Si1 0.5(9) . .
O21 W6 O13 W2 44(2) . .
O9 W6 O13 W2 -89.2(8) . .
O5 W6 O13 W2 -2.6(8) . .
O15 W6 O13 W2 -177.8(7) . .
O8 W6 O13 W2 98.1(10) . .
O4 W6 O13 W2 -137.2(12) . .
O21 W6 O13 W5 -54(2) . .
O9 W6 O13 W5 173.4(7) . .
O5 W6 O13 W5 -99.9(9) . .
O15 W6 O13 W5 84.9(8) . .
O8 W6 O13 W5 0.8(8) . .
O4 W6 O13 W5 125.5(12) . .
C9 N3 C13 C16 -150(3) . 2_675
C11 N3 C13 C16 51(4) . 2_675
C1 C8 C14 C10 -5(4) . .
C9 C8 C14 C10 -180(3) . .
C7 C10 C14 C8 7(5) . .
O14 Si1 O14 O4 -138(12) 2_665 2_665
O4 Si1 O14 O4 180.001(4) . 2_665
O12 Si1 O14 O4 123.4(14) 2_665 2_665
O12 Si1 O14 O4 -56.6(14) . 2_665
O13 Si1 O14 O4 -119.7(14) . 2_665
O13 Si1 O14 O4 60.3(14) 2_665 2_665
O14 Si1 O14 W1 -139(12) 2_665 2_665
O4 Si1 O14 W1 -1.2(13) 2_665 2_665
O4 Si1 O14 W1 178.8(13) . 2_665
O12 Si1 O14 W1 122.2(17) 2_665 2_665
O12 Si1 O14 W1 -57.8(17) . 2_665
O13 Si1 O14 W1 -121.0(17) . 2_665
O13 Si1 O14 W1 59.0(17) 2_665 2_665
O14 Si1 O14 W4 97(12) 2_665 2_665
O4 Si1 O14 W4 -125.2(18) 2_665 2_665
O4 Si1 O14 W4 54.8(18) . 2_665
O12 Si1 O14 W4 -1.8(12) 2_665 2_665
O12 Si1 O14 W4 178.2(12) . 2_665
O13 Si1 O14 W4 115.0(16) . 2_665
O13 Si1 O14 W4 -65.0(16) 2_665 2_665
O14 Si1 O14 W2 -19(12) 2_665 .
O4 Si1 O14 W2 119.4(16) 2_665 .
O4 Si1 O14 W2 -60.6(16) . .
O12 Si1 O14 W2 -117.2(14) 2_665 .
O12 Si1 O14 W2 62.8(14) . .
O13 Si1 O14 W2 -0.4(11) . .
O13 Si1 O14 W2 179.6(11) 2_665 .
O23 W2 O14 Si1 179.6(14) . .
O10 W2 O14 Si1 -130.6(15) 2_665 .
O17 W2 O14 Si1 -45.1(14) . .
O16 W2 O14 Si1 127.9(15) . .
O5 W2 O14 Si1 43.7(14) . .
O13 W2 O14 Si1 0.3(10) . .
O23 W2 O14 O4 -108(2) . 2_665
O10 W2 O14 O4 -58.5(16) 2_665 2_665
O17 W2 O14 O4 26.9(18) . 2_665
O16 W2 O14 O4 -160.0(19) . 2_665
O5 W2 O14 O4 115.8(17) . 2_665
O13 W2 O14 O4 72.4(17) . 2_665
O23 W2 O14 W1 -45(2) . 2_665
O10 W2 O14 W1 5.0(6) 2_665 2_665
O17 W2 O14 W1 90.4(8) . 2_665
O16 W2 O14 W1 -96.6(8) . 2_665
O5 W2 O14 W1 179.3(7) . 2_665
O13 W2 O14 W1 135.9(12) . 2_665
O23 W2 O14 W4 49(2) . 2_665
O10 W2 O14 W4 98.7(8) 2_665 2_665
O17 W2 O14 W4 -175.9(7) . 2_665
O16 W2 O14 W4 -2.9(6) . 2_665
O5 W2 O14 W4 -87.0(7) . 2_665
O13 W2 O14 W4 -130.4(12) . 2_665
N3 C11 C15 N4 54(3) . 2_675
O19 W1 O15 W6 157.0(15) . .
O6 W1 O15 W6 -100.0(16) . .
O10 W1 O15 W6 -15(3) . .
O11 W1 O15 W6 57.5(16) . .
O4 W1 O15 W6 -4.9(14) . .
O14 W1 O15 W6 -36.0(16) 2_665 .
O21 W6 O15 W1 -159.1(16) . .
O9 W6 O15 W1 -58.1(16) . .
O5 W6 O15 W1 24(3) . .
O8 W6 O15 W1 102.4(16) . .
O13 W6 O15 W1 37.2(16) . .
O4 W6 O15 W1 4.8(13) . .
O23 W2 O16 W4 -156.5(14) . 2_665
O10 W2 O16 W4 -54.8(15) 2_665 2_665
O17 W2 O16 W4 24(3) . 2_665
O5 W2 O16 W4 104.2(15) . 2_665
O13 W2 O16 W4 39.6(15) . 2_665
O14 W2 O16 W4 5.5(13) . 2_665
C6 N4 C16 C13 136(3) . 2_675
C15 N4 C16 C13 -61(4) 2_675 2_675
O1 W5 O17 W2 155.4(17) . .
O8 W5 O17 W2 54.2(19) . .
O7 W5 O17 W2 -39(3) . .
O2 W5 O17 W2 -108.0(19) 2_665 .
O13 W5 O17 W2 -9.1(15) . .
O12 W5 O17 W2 -46.1(18) . .
O23 W2 O17 W5 -152.6(17) . .
O10 W2 O17 W5 105.7(18) 2_665 .
O16 W2 O17 W5 27(3) . .
O5 W2 O17 W5 -53.2(19) . .
O13 W2 O17 W5 9.3(15) . .
O14 W2 O17 W5 43.6(18) . .
O18 W3 O20 W4 157.2(18) . 2_665
O11 W3 O20 W4 -22(4) . 2_665
O9 W3 O20 W4 -102.3(19) . 2_665
O2 W3 O20 W4 57.7(19) . 2_665
O12 W3 O20 W4 -4.4(16) 2_665 2_665
O4 W3 O20 W4 -36.6(19) . 2_665
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.000 0.500 0.500 148 35 ' '
